A facile approach to a silver conductive ink with high performance for macroelectronics
© Tao et al.; licensee Springer. 2013
Received: 22 March 2013
Accepted: 23 May 2013
Published: 25 June 2013
An unusual kind of transparent and high-efficiency organic silver conductive ink (OSC ink) was synthesized with silver acetate as silver carrier, ethanolamine as additive, and different kinds of aldehyde-based materials as reduction agents and was characterized by using a thermogravimetric analyzer, X-ray diffraction, a scanning electron microscope, and a four-point probe. The results show that different reduction agents all have an important influence on the conductive properties of the ink through a series of complex chemical reactions, and especially when formic acid or dimethylformamide was used as the reduction agent and sintered at 120°C for 30 s, the resistivity can be lowered to 6 to 9 μΩ·cm. Furthermore, formula mechanism, conductive properties, temperature, and dynamic fatigue properties were investigated systematically, and the feasibility of the OSC ink was also verified through the preparation of an antenna pattern.
KeywordsOrganic silver conductive ink (OSC ink) Conductive pattern Formula mechanism Antenna pattern
Most research efforts in macroelectronics have opened the door for the manufacture of lightweight, flexible, cost-effective electronic devices that are beyond the conventional silicon-based devices, including flexible displays, flexible and conformal antenna arrays, electronic solar cell arrays, radio-frequency identification tags, flexible batteries, electronic circuits fabricated in clothing, and biomedical devices. Usually, most of them require electrical contacts.
Up to now, various materials such as conjugated polymers, graphene, carbon nanotubes, and metals have been used for the preparation of electrodes and conductive patterns using solution processing methods[8–11]. Specifically, metal nanoparticle inks have attracted more and more attention due to their high conductivity and thermal stability after having been sintered[12–14].
However, metallic nanoparticle inks often require high annealing temperatures (>150°C) to decompose stabilizing agents and other polymeric additives that inhibit electrical conductivity, with the high annealing temperature limiting the choice of substrate. Besides, they still cannot completely avoid the condensation and agglomeration of nanoparticles, especially after long-term storage. The agglomerated particles may damage the equipment and influence the printing quality. During preparation, a high-speed centrifuge or vacuum dryer must be used to take nanometal particles out, so these inks cannot be produced on a large scale. All of these will cause a higher production cost[15–18].
There is no surprise to the fact that organic silver conductive ink (OSC ink) has received increasing attention as a potentially much lower cost alternative[19–21]. This kind of ink mainly consists of a silver carrier, weak reduction agent, solvent, and additives, and a continuous conductive silver track can be fabricated during the sintering process. This strategy can compensate for the lack of conductive metal nanoink and thus becomes the development direction of conductive ink for macroelectronics[22–25].
In our previous research, the relationship between different kinds of amines and ink properties was investigated systematically. The addition of different amines not only increased the solid content of the conductive ink but also decreased the sintering temperature by complexation[26–28].
Here, based on the previous results, the formula of the conductive ink will be further optimized using silver acetate as silver carrier, ethanolamine as additive, and different kinds of organic aldehyde as reduction agents, such as ethylene glycol, acetaldehyde, formic acid, dimethylformamide, and glucose. Furthermore, the formula mechanism, conductive properties, temperature, dynamic fatigue properties, and feasibility verification of the OSC ink through the preparation of an antenna pattern were also investigated systematically[29–31].
Silver acetate was obtained from Shanghai Lingfeng Chemical Reagent Co., Ltd. (Shanghai, China). Polydimethylsiloxane (PDMS) including base and curing agents was obtained from Dow Corning Co. (Midland, MI, USA; SYLGARD 184 silicone elastomer). Polyester film (0.1 ± 0.02 mm) came from Shanghai Weifen Industry Co., Ltd (Shanghai, China). Ethylene glycol, acetaldehyde, formic acid, dimethylformamide, glucose, ethyl alcohol, and other solvents were of analytical grade and used without further purification. Deionized water was used in all experimental processes.
Synthesis of OSC ink
For the preparation of conductive ink (1 g), silver acetate (0.32 g; which means if all silver ions are reduced to elemental silver, the content of elemental silver is 20 wt.%) and ethanolamine (0.2 g) were added to ethanol (0.13 g) and different reduction agents (0.35 g; ethylene glycol, acetaldehyde, formic acid, dimethylformamide, or glucose, etc.) under vigorous stirring until a transparent solution was obtained.
Preparation of antenna pattern
For the preparation of the PDMS pattern as template, polyethylene terephthalate (PET) was adhered to a sheet glass using both side tapes, and 3-g PDMS (base/curing agent is 15/1) was dropped on the center of the PET film. Then, after spin coating (800 rpm), baking at 80°C for 3 h, and laser etching, the desired PDMS pattern as template can be fabricated with the conductive track (a thickness of 200 μm and a width of 200 μm).
For the preparation of the antenna pattern, the synthesized OSC ink was dropped into the trench of the PDMS template track using a syringe, and the ink will flow to all of the track spontaneously until full; then, it will be sintered at 120°C for 30 s. Finally, the PDMS template can be peeled off easily by forceps, and the desired antenna pattern was achieved.
OSC ink was characterized by using a Ubbelohde viscometer (CN60M, Zxyd Technology Co., Ltd., Beijing, China); a surface tension instrument (A101, Kino Industry Co., Ltd, New York, USA); X-ray diffraction (XRD; max 2550 PC, Rigaku-D, Rigaku Corporation, Tokyo, Japan) using Cu Kα radiation; scanning electron microscopy (SEM; S-360, Cambridge Instruments Ltd., Cambridge, England) operated at 10 kV; thermogravimetric analysis (TGA; QS-500, TA Instruments Inc., New Castle, DE, USA) with a heating rate of 5°C·min−1 in a nitrogen atmosphere; a four-point probe equipped with a semiconductor characterization system (BD-90, Shanghai Power Tool Institute, Shanghai, China); a memory hicorder (8870–20, HIOKI, Nagano, Japan) with a heating device from room temperature to 120°C, a steady current mechanism (10 mA), and an amplifier (×100); and a dynamic fatigue tester (built in the lab) with steady current mechanism (10 mA). The antenna pattern was investigated using a Uscan explorer with 3D profilometer system (D46047, Nanofocus, Oberhausen, Germany).
Results and discussion
In this formula, silver acetate was chosen as silver carrier, which can control the reaction rate effectively by adjusting the concentration of the silver ion in the mixing solvent because of its worse solubility. Ethanolamine was used to increase the silver content of the conductive ink to guarantee the conductivity and further to decrease the sintering temperature.
OSC ink properties
The thermal properties of the prepared OSC ink were investigated by TGA with a heating rate of 5°C/min, as depicted in Figure 3a. It can be seen that there exists an evident mass-decreasing area, from 80°C to 160°C, which is related to the evaporation of organic materials; finally, 20.3 wt.% of the mass remains, which indicates that the ink contains 20.3 wt.% silver and agrees well with the calculated value (20 wt.%). If several drops of ammonia were added, the solid content can be further increased to 28 wt.% at most because of its stronger coordination ability than ethanolamine. However, more ammonia will cause the instability of the conductive ink due to its volatilization.
The conductive properties of the prepared OSC ink were investigated using different sintering temperatures (90°C, 120°C, 150°C) for different durations of time (from 0 to 60 min), which also can be explained by percolation theory, as shown in Figure 3b. During the sintering process, initially, there are only silver acetate and silver oxide, without any elemental silver, so there is no conductivity. Then, almost all of the silver oxide was reduced to elemental silver at the same time, indicating that a continuous conductive track has been fabricated and showing metallic luster and high conductivity. Especially, based on the present formula of the ink, when the sintering temperature is 120°C for 30 s, the resistivity can drop to 7 to 9 μΩ·cm.
Figure 3c shows an XRD pattern of the silver ink after sintering, and all diffraction peaks could be indexed to the face-centered cubic phase of silver. The lattice constant calculated from this XRD pattern was 4.098, which was very close to the reported data (a = 4.0862, JCPDS file no. 04–0783). The inset is the surface morphology of the conductive ink after sintering, and more information also can be seen from Figure 3d.
Temperature and dynamic fatigue properties
From Figure 4a,b, a set of equipment including a heating device from room temperature to 120°C, steady current mechanism (10 mA), amplifier (×100), memory hicorder (HIOKI, 8870–20), etc. were assembled together, aiming at monitoring the changes of the resistivity of the conductive silver line during the heating and cooling processes. It can be obtained that between 20°C and 100°C, the largest variable quantity of the resistivity is just about 0.28 Ω. After linear fitting, the slopes of the heating curve and the cooling curve, which can be called temperature coefficient of resistance (TCR), approximately have the same slope (kh = kc = 0.0007 aR/°C−1), indicating the good thermal stability of the conductive silver line. The TCR is a little different compared with the TCR of bulk silver (0.0038 aR/°C−1). This phenomenon is mainly caused by the complex microstructure of the silver thin film which will bring more barriers during the electron-transfer process. Moreover, it also can be seen that though the heating curve and cooling curve have the same TCR, the cooling curve is always below the heating curve. This is mainly because the natural cooling process (about 28 min) needs more time than the heating process (15 min).
From Figure 4c, a bending tester was used to study the dynamic fatigue of the PET-based conductive silver line. During the test, the conductive line makes a periodic bending movement from I to V, and every period needs 2 s. The details also can be seen from the set in Figure 3b. It is very interesting to find that the resistivity of the conductive silver lines also increases with the increase of the bending angle. From I to III, the resistivity increases from 5.2 to 5.76 Ω. It can be explained that when bending, the silver thin film was stretched and became thin, especially on the top point of the conductive line, so the stack density and conductivity decreased. From III to V, the resistivity was back to 5.2 Ω, and after a periodic movement like this for 1,000 times, the resistivity did not significantly increase due to the good ductility of the metal silver. Generally speaking, compared with other printing technologies, this method also shows good adhesion between the silver thin film and PET, showing good results.
Preparation of an antenna pattern
The thin film PDMS pattern with a thickness of 200 μm, a width of 200 μm, and a total length of 15.8 cm on the PET substrate was prepared using a laser and used as template. The synthesized OSC ink with blue dye (seen more clearly) was dropped to the center of the template using a syringe (20 μL per drop). Due to the good wetting and film-forming ability of the ink, it will flow along the template track until it fills the whole track, especially after plasma treatment with oxygen. After sintering at 120°C for 30 s, the continuous conductive track can be fabricated, and the total resistor Rab decreased to 4.6 Ω measured by a multimeter (middle image of Figure 5) with a width of 200 μm and thickness of 22 μm according to the surface profile.
In summary, an unusual kind of high-efficiency, transparent organic silver conductive ink (OSC ink) was synthesized with silver acetate as silver carrier, ethanolamine as additive, and different kinds of aldehyde-based materials as reduction agents successfully. The results show that different reduction agents have an important influence on the ink properties through a series of complex chemical reactions, and when formic acid or dimethylformamide was used as the reduction agent and sintered at 120°C for 30 s, the resistivity can be lowered down to 6 to 9 μΩ·cm. It also can be obtained that the fabricated conductive pattern shows good temperature and dynamic fatigue properties. Besides, the feasibility of the synthesized OSC ink was verified through the preparation of an antenna pattern using drop or fit-to-flow method successfully.
This work was supported by the project funded by the Priority Academic Program Development of Jiangsu Higher Education Institutions (PAPD).
- Chen Y, Au J, Kazlas P, Ritenour A, Gates H, McCreary M: Flexible active-matrix electronic ink display. Nature 2003, 423: 136.View Article
- Bairavasubramanian R, Thompson D, Ponchak GE, Tentzeris MM, Papapolymero-u J: Liquid crystal polymer (LCP): a new organic material for the development of multilayer dual-frequency/dual-polarization flexible antenna arrays. IEEE Anten Wirel Pr 2005, 4: 22–26. 10.1109/LAWP.2004.841626View Article
- Otte K, Makhova L, Braun A, Konovalov I: Flexible Cu(In, Ga) Se2 thin-film solar cells for space application. Thin Solid Films 2006, 511: 613–622.View Article
- Baeg KJ, Khim D, Kim J, Yang BD, Kang M, Jung SW: High-performance top-gated organic field-effect transistor memory using electrets for monolithic printed flexible NAND flash memory. Adv Funct Mater 2012, 22: 2915–2926. 10.1002/adfm.201200290View Article
- Nishide H, Oyaizu K: Toward flexible batteries. Science 2008, 319: 737–738. 10.1126/science.1151831View Article
- Meng Y, Zhao Y, Hu C, Cheng H, Hu Y, Zhang Z, Shi G, Qu L: All-graphene core-sheath microfibers for all-solid-state, stretchable fibriform supercapacitors and wearable electronic textiles. Adv Mater 2013, 25: 2326–2331. 10.1002/adma.201300132View Article
- Cha C, Shin SR, Annabi N, Dokmeci MR, Khademhosseini A: Carbon-based nanomaterials: multifunctional materials for biomedical engineering. ACS Nano 2013, 7: 2891–2897. 10.1021/nn401196aView Article
- Wang JZ, Zheng ZH, Li HW, Huck WTS, Sirringhaus H: Dewetting of conducting polymer inkjet droplets on patterned surfaces. Nat Mater 2004, 3: 171–176. 10.1038/nmat1073View Article
- Huang X, Qi X, Boey F, Zhang H: Graphene-based composites. Chem Soc Rev 2012, 41: 666–686. 10.1039/c1cs15078bView Article
- Mensing JP, Kerdcharoen T, Sriprachuabwong C, Wisitsoraat A, Phokharatkul D, Lomas T: Facile preparation of graphene–metal phthalocyanine hybrid material by electrolytic exfoliation. J Mater Chem 2012, 22: 17094–17099. 10.1039/c2jm32588hView Article
- Wu L, Li Y, Ong BS: Printed silver ohmic contacts for high-mobility organic thin-film transistors. J Am Chem Soc 2006, 128: 4202–4203. 10.1021/ja058725wView Article
- Choi CS, Jo YH, Kim MG, Lee HM: Control of chemical kinetics for sub-10 nm Cu nanoparticles to fabricate highly conductive ink below 150°C. Nanotechnology 2012, 23: 065601–065609. 10.1088/0957-4484/23/6/065601View Article
- Russo A, Ahn BY, Adams JJ, Duoss EB, Bernhard JT, Lewis JA: Pen-on-paper flexible electronics. Adv Mater 2011, 23: 3426–3430. 10.1002/adma.201101328View Article
- Hösel M, Krebs FC: Large-scale roll-to-roll photonic sintering of flexo printed silver nanoparticle electrodes. J Mater Chem 2012, 22: 15683–15688. 10.1039/c2jm32977hView Article
- Kim J, Kang SW, Mun SH, Kang YS: Facile synthesis of copper nanoparticles by ionic liquids and its application to facilitated olefin transport membranes. Ind Eng Chem Res 2009, 48: 7437–7441. 10.1021/ie900150cView Article
- Li Y, Wu Y, Ong BS: Facile synthesis of silver nanoparticles useful for fabrication of high-conductivity elements for printed electronics. J Am Chem Soc 2005, 127: 3266–3267. 10.1021/ja043425kView Article
- Hussain I, Graham S, Wang Z, Tan B, Sherrington DC, Rannard SP: Size-controlled synthesis of near-monodisperse gold nanoparticles in the 1–4 nm range using polymeric stabilizers. J Am Chem Soc 2005, 127: 16398–16399. 10.1021/ja055321vView Article
- Chen S, Carroll DL: Silver nanoplates: size control in two dimensions and formation mechanisms. J Phys Chem B 2004, 108: 5500–5506. 10.1021/jp031077nView Article
- Walker SB, Lewis JA: Reactive silver inks for patterning high-conductivity features at mild temperatures. J Am Chem Soc 2012, 134: 1419–1421. 10.1021/ja209267cView Article
- Wu JT, Hsu SLC, Tsai MH, Hwang WS: Direct inkjet printing of silver nitrate/poly( N -vinyl-2-pyrrolidone) inks to fabricate silver conductive lines. J Phys Chem C 2010, 114: 4659–4662. 10.1021/jp100326kView Article
- Rickerby J, Simon A, Jeynes C, Morgan TJ, Steinke JHG: 1,1,1,5,5,5-Hexafluoroacetylacetonate copper(I) poly(vinylsiloxane)s as precursors for copper direct-write. Chem Mater 2006, 18: 2489–2498. 10.1021/cm052103sView Article
- Wu Y, Li Y, Ong BS: A simple and efficient approach to a printable silver conductor for printed electronics. J Am Chem Soc 2007, 129: 1862–1863. 10.1021/ja067596wView Article
- Hiraoka M: Ink-jet printing of organic metal electrodes using charge-transfer compounds. Appl Phys Lett 2006, 89: 173504–173507. 10.1063/1.2363178View Article
- Gamerith S, Klug A, Scheiber H, Scherf U, Moderegger E, List EJW: Direct ink-jet printing of Ag–Cu nanoparticle and Ag-precursor based electrodes for OFET applications. Adv Funct Mater 2007, 17: 3111–3118. 10.1002/adfm.200600762View Article
- Moonen PF, Yakimets I, Huskens J: Fabrication of transistors on flexible substrates: from mass-printing to high-resolution alternative lithography strategies. Adv Mater 2012, 24: 5526–5541. 10.1002/adma.201202949View Article
- Chang Y, Wang DY, Tai YL, Yang ZG: Preparation, characterization and reaction mechanism of a novel silver-organic conductive ink. J Mater Chem 2012, 22: 25296–25301. 10.1039/c2jm34569bView Article
- Li Y, Sun H, Chu H: Controlled preparation of inorganic nanostructures on substrates by dip-pen nanolithography. Chem Asian J 2010, 5: 980–990. 10.1002/asia.200900681View Article
- Tai YL, Yang ZG, Li ZD: A promising approach to conductive patterns with high efficiency for flexible electronics. Appl Surf Sci 2011, 257: 7096–7100. 10.1016/j.apsusc.2011.03.056View Article
- Tai YL, Yang ZG: Fabrication of paper-based conductive patterns for flexible electronics by direct-writing. J Mater Chem 2011, 21: 5938–5943. 10.1039/c0jm03065aView Article
- Dearden AL, Smith PJ, Shin DY, Reis N, Derby B, O’Brien P: A low curing temperature silver ink for use in ink-jet printing and subsequent production of conductive tracks. Macromol Rapid Commun 2005, 26: 315–318. 10.1002/marc.200400445View Article
- Perelaer J, Smith PJ, Mager D, Soltman D, Volkman SK, Subramanian V, Korvinkdf JG, Schubert US: Printed electronics: the challenges involved in printing devices, interconnects, and contacts based on inorganic materials. J Mater Chem 2010, 20: 8446–8453. 10.1039/c0jm00264jView Article
- Tao Y, Tao YX, Wang L, Wang B, Yang ZG, Tai YL: High-reproducibility, flexible conductive patterns fabricated with silver nanowire by drop or fit-to-flow method. Nanoscale Res Lett 2013, 8: 147–152. 10.1186/1556-276X-8-147View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.